#------------------------------------------------------------------------------
#$Date: 2016-03-26 02:56:09 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180161 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/57/7105729.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7105729
loop_
_publ_author_name
'Andrea Alsobrook'
'Brad Hauser'
'Joseph Hupp'
'Evgeny V.Alekseev'
'Wulf Depmeier'
'Thomas Albrecht-Schmitt'
_publ_section_title
;
 Cubic and rhombohedral heterobimetallic networks constructed from
 uranium, transition metals, and phosphonoacetate: new methods for
 constructing porous materials
;
_journal_name_full               Chem.Commun.
_journal_page_first              9167
_journal_paper_doi               10.1039/c0cc03507f
_journal_volume                  46
_journal_year                    2010
_chemical_formula_moiety         Co2[(UO2)6(PO3CH2CO2)3O3(OH)(H2O)2]*16H2O
_chemical_formula_sum            'C6 H42 Co2 O49 P3 U6'
_chemical_formula_weight         2537.35
_chemical_name_systematic
;
?
;
_space_group_IT_number           204
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   26.3861(3)
_cell_length_b                   26.3861(3)
_cell_length_c                   26.3861(3)
_cell_measurement_reflns_used    3461
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.48
_cell_measurement_theta_min      1.89
_cell_volume                     18370.7(4)
_computing_cell_refinement       'SMART, SAINT'
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'BRUKER APEX'
_diffrn_measurement_method       '0.3 /w wxposure'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0493
_diffrn_reflns_av_sigmaI/netI    0.0133
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -34
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            110457
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         1.89
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count na
_diffrn_standards_interval_time  na
_diffrn_standards_number         na
_exptl_absorpt_coefficient_mu    22.012
_exptl_absorpt_correction_T_max  0.683
_exptl_absorpt_correction_T_min  0.274
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELXPREP
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    3.670
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    .
_exptl_crystal_description       block
_exptl_crystal_F_000             17936
_exptl_crystal_size_max          0.08715
_exptl_crystal_size_mid          0.05055
_exptl_crystal_size_min          0.01730
_refine_diff_density_max         1.002
_refine_diff_density_min         -1.357
_refine_diff_density_rms         0.150
_refine_ls_extinction_coef       0
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     241
_refine_ls_number_reflns         3763
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.076
_refine_ls_R_factor_all          0.0209
_refine_ls_R_factor_gt           0.0176
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0176P)²+226.1683P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0420
_refine_ls_wR_factor_ref         0.0429
_reflns_number_gt                3461
_reflns_number_total             3763
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            C0CC03507F.TXT
_cod_data_source_block           Co2[(UO2)6(PO3CH2CO2)3O3(OH)(H2O)2]*16H2O
_cod_database_code               7105729
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.069577(6) 0.364696(7) 0.0000 0.01063(4) Uani 1 2 d S . .
U2 U 0.0000 0.350441(6) 0.131630(6) 0.00723(4) Uani 1 2 d S . .
U3 U 0.071558(5) 0.347245(5) 0.261491(4) 0.00958(3) Uani 1 1 d . . .
Co1 Co 0.0000 0.5000 0.14032(3) 0.01160(19) Uani 1 4 d S . .
Co2 Co 0.18721(3) 0.18721(3) 0.18721(3) 0.0289(3) Uani 0.75 3 d SP . .
Co3 Co 0.2500 0.2500 0.2500 0.0246(3) Uani 1 6 d S . .
P1 P 0.12444(3) 0.35657(3) 0.13238(3) 0.01081(18) Uani 1 1 d . . .
C1 C 0.16934(13) 0.30770(14) 0.11539(13) 0.0163(8) Uani 1 1 d . . .
H2A H 0.1517 0.2757 0.1115 0.020 Uiso 1 1 calc R . .
H2B H 0.1849 0.3161 0.0832 0.020 Uiso 1 1 calc R . .
C2 C 0.21009(13) 0.30235(13) 0.15560(13) 0.0132(7) Uani 1 1 d . . .
O1 O 0.15402(9) 0.40226(10) 0.14864(10) 0.0174(6) Uani 1 1 d . . .
O2 O 0.08895(9) 0.33597(10) 0.17353(9) 0.0147(5) Uani 1 1 d . . .
O3 O 0.08842(9) 0.36601(11) 0.08813(9) 0.0196(6) Uani 1 1 d . . .
O4 O 0.23990(9) 0.33851(9) 0.16282(10) 0.0151(5) Uani 1 1 d . . .
O5 O 0.21239(10) 0.26171(10) 0.18061(10) 0.0197(6) Uani 1 1 d . . .
O6 O 0.08820(15) 0.29972(15) 0.0000 0.0246(9) Uani 1 2 d S . .
O7 O 0.05762(14) 0.43180(14) 0.0000 0.0185(8) Uani 1 2 d S . .
O8 O 0.0000 0.28209(13) 0.12703(13) 0.0144(8) Uani 1 2 d S . .
O9 O 0.0000 0.41942(13) 0.13703(13) 0.0139(8) Uani 1 2 d S . .
O10 O 0.06661(10) 0.27945(10) 0.26776(10) 0.0198(6) Uani 1 1 d . . .
O11 O 0.07931(10) 0.41449(9) 0.25377(10) 0.0180(6) Uani 1 1 d . . .
O12 O 0.0000 0.35240(15) 0.04882(13) 0.0176(8) Uani 1 2 d S . .
O13 O 0.15630(14) 0.39553(16) 0.0000 0.0231(9) Uani 1 2 d S . .
O14 O 0.0000 0.34755(14) 0.21473(13) 0.0140(8) Uani 1 2 d S . .
O15 O 0.0000 0.3604(2) 0.31190(15) 0.0358(12) Uani 1 2 d S . .
OW1 O 0.0422(3) 0.5000 0.2052(3) 0.0235(19) Uani 0.50 2 d SP . .
OW1A O 0.0672(3) 0.5000 0.1858(3) 0.0186(17) Uani 0.50 2 d SP . .
OW2 O 0.0547(2) 0.5000 0.0850(2) 0.0746(18) Uani 1 2 d S . .
OW3 O 0.13503(12) 0.13503(12) 0.13503(12) 0.075(2) Uani 1 3 d S . .
OW4 O 0.11213(16) 0.2053(2) 0.1719(2) 0.0805(16) Uani 1 1 d . . .
OW5 O 0.24213(19) 0.3455(2) 0.0000 0.0460(13) Uani 1 2 d S . .
OW6 O 0.1811(4) 0.5000 0.0227(3) 0.039(2) Uani 0.50 2 d SP . .
OW7 O 0.0225(4) 0.2098(4) 0.2020(3) 0.084(3) Uani 0.50 1 d P . .
OW8 O 0.1182(7) 0.2010(7) 0.0000 0.099(5) Uiso 0.50 2 d SP . .
OW9 O 0.0000 0.2210(10) 0.0397(10) 0.060(6) Uiso 0.25 2 d SP . .
OW10 O 0.0646(8) 0.1724(8) 0.0910(8) 0.078(6) Uiso 0.25 1 d P . .
OW11 O 0.0227(6) 0.2044(6) 0.0572(6) 0.053(4) Uiso 0.25 1 d P . .
OW12 O 0.0866(10) 0.0866(10) 0.0866(10) 0.105(14) Uiso 0.25 3 d SP . .
OW13 O 0.1134(11) 0.1740(11) 0.0571(11) 0.123(9) Uiso 0.25 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 U1 O7 174.11(17) . . ?
O6 U1 O12 94.91(15) . 26 ?
O7 U1 O12 89.93(14) . 26 ?
O6 U1 O12 94.91(15) . . ?
O7 U1 O12 89.93(14) . . ?
O12 U1 O12 69.28(14) 26 . ?
O6 U1 O3 87.50(7) . . ?
O7 U1 O3 91.28(7) . . ?
O12 U1 O3 136.66(9) 26 . ?
O12 U1 O3 67.40(9) . . ?
O6 U1 O3 87.50(7) . 26 ?
O7 U1 O3 91.28(7) . 26 ?
O12 U1 O3 67.40(9) 26 26 ?
O12 U1 O3 136.66(9) . 26 ?
O3 U1 O3 155.80(12) . 26 ?
O6 U1 O13 93.58(16) . . ?
O7 U1 O13 80.53(15) . . ?
O12 U1 O13 144.22(8) 26 . ?
O12 U1 O13 144.22(8) . . ?
O3 U1 O13 78.35(6) . . ?
O3 U1 O13 78.35(6) 26 . ?
O6 U1 U1 106.00(13) . 3 ?
O7 U1 U1 79.90(12) . 3 ?
O12 U1 U1 35.89(7) 26 3 ?
O12 U1 U1 35.89(7) . 3 ?
O3 U1 U1 102.07(6) . 3 ?
O3 U1 U1 102.07(6) 26 3 ?
O13 U1 U1 160.43(10) . 3 ?
O6 U1 U2 92.10(6) . 26 ?
O7 U1 U2 90.70(6) . 26 ?
O12 U1 U2 27.03(7) 26 26 ?
O12 U1 U2 96.30(7) . 26 ?
O3 U1 U2 163.57(6) . 26 ?
O3 U1 U2 40.37(6) 26 26 ?
O13 U1 U2 118.050(8) . 26 ?
U1 U1 U2 62.278(2) 3 26 ?
O6 U1 U2 92.10(6) . . ?
O7 U1 U2 90.70(6) . . ?
O12 U1 U2 96.30(7) 26 . ?
O12 U1 U2 27.03(7) . . ?
O3 U1 U2 40.37(6) . . ?
O3 U1 U2 163.57(6) 26 . ?
O13 U1 U2 118.050(8) . . ?
U1 U1 U2 62.278(2) 3 . ?
U2 U1 U2 123.301(5) 26 . ?
O8 U2 O9 179.37(15) . . ?
O8 U2 O12 87.51(15) . . ?
O9 U2 O12 93.12(15) . . ?
O8 U2 O14 91.86(15) . . ?
O9 U2 O14 87.51(14) . . ?
O12 U2 O14 179.37(14) . . ?
O8 U2 O2 83.28(7) . 28 ?
O9 U2 O2 96.44(7) . 28 ?
O12 U2 O2 115.14(5) . 28 ?
O14 U2 O2 64.76(5) . 28 ?
O8 U2 O2 83.28(7) . . ?
O9 U2 O2 96.44(7) . . ?
O12 U2 O2 115.14(5) . . ?
O14 U2 O2 64.76(5) . . ?
O2 U2 O2 127.03(10) 28 . ?
O8 U2 O3 97.26(8) . 28 ?
O9 U2 O3 83.02(8) . 28 ?
O12 U2 O3 63.92(6) . 28 ?
O14 U2 O3 116.18(6) . 28 ?
O2 U2 O3 54.07(7) 28 28 ?
O2 U2 O3 178.86(8) . 28 ?
O8 U2 O3 97.26(8) . . ?
O9 U2 O3 83.02(8) . . ?
O12 U2 O3 63.92(6) . . ?
O14 U2 O3 116.18(6) . . ?
O2 U2 O3 178.86(8) 28 . ?
O2 U2 O3 54.07(7) . . ?
O3 U2 O3 124.82(11) 28 . ?
O8 U2 P1 92.837(16) . 28 ?
O9 U2 P1 87.161(16) . 28 ?
O12 U2 P1 90.278(16) . 28 ?
O14 U2 P1 89.753(16) . 28 ?
O2 U2 P1 27.21(5) 28 28 ?
O2 U2 P1 153.97(5) . 28 ?
O3 U2 P1 27.09(5) 28 28 ?
O3 U2 P1 151.66(6) . 28 ?
O8 U2 P1 92.837(16) . . ?
O9 U2 P1 87.161(16) . . ?
O12 U2 P1 90.278(16) . . ?
O14 U2 P1 89.753(16) . . ?
O2 U2 P1 153.97(5) 28 . ?
O2 U2 P1 27.21(5) . . ?
O3 U2 P1 151.66(6) 28 . ?
O3 U2 P1 27.09(5) . . ?
P1 U2 P1 174.32(3) 28 . ?
O8 U2 U3 92.14(10) . . ?
O9 U2 U3 87.32(9) . . ?
O12 U2 U3 151.151(2) . . ?
O14 U2 U3 28.854(3) . . ?
O2 U2 U3 93.42(5) 28 . ?
O2 U2 U3 36.47(5) . . ?
O3 U2 U3 144.37(5) 28 . ?
O3 U2 U3 87.57(5) . . ?
P1 U2 U3 118.535(15) 28 . ?
P1 U2 U3 60.914(15) . . ?
O8 U2 U3 92.14(10) . 28 ?
O9 U2 U3 87.32(9) . 28 ?
O12 U2 U3 151.151(2) . 28 ?
O14 U2 U3 28.854(3) . 28 ?
O2 U2 U3 36.47(5) 28 28 ?
O2 U2 U3 93.42(5) . 28 ?
O3 U2 U3 87.57(5) 28 28 ?
O3 U2 U3 144.37(5) . 28 ?
P1 U2 U3 60.914(15) 28 28 ?
P1 U2 U3 118.535(15) . 28 ?
U3 U2 U3 57.698(4) . 28 ?
O11 U3 O10 177.31(13) . . ?
O11 U3 O14 91.70(12) . . ?
O10 U3 O14 89.60(12) . . ?
O11 U3 O15 90.58(16) . . ?
O10 U3 O15 92.09(16) . . ?
O14 U3 O15 68.55(11) . . ?
O11 U3 O1 91.64(11) . 45 ?
O10 U3 O1 88.85(11) . 45 ?
O14 U3 O1 140.29(9) . 45 ?
O15 U3 O1 71.86(10) . 45 ?
O11 U3 O2 89.47(10) . . ?
O10 U3 O2 88.83(10) . . ?
O14 U3 O2 68.23(9) . . ?
O15 U3 O2 136.76(10) . . ?
O1 U3 O2 151.35(8) 45 . ?
O11 U3 O4 89.71(10) . 45 ?
O10 U3 O4 87.89(11) . 45 ?
O14 U3 O4 145.47(9) . 45 ?
O15 U3 O4 145.96(10) . 45 ?
O1 U3 O4 74.10(8) 45 45 ?
O2 U3 O4 77.28(8) . 45 ?
O11 U3 U3 96.54(9) . 28 ?
O10 U3 U3 85.84(9) . 28 ?
O14 U3 U3 33.16(7) . 28 ?
O15 U3 U3 36.05(8) . 28 ?
O1 U3 U3 107.20(6) 45 28 ?
O2 U3 U3 101.10(6) . 28 ?
O4 U3 U3 173.56(6) 45 28 ?
O11 U3 U2 86.24(8) . . ?
O10 U3 U2 93.83(8) . . ?
O14 U3 U2 28.00(7) . . ?
O15 U3 U2 96.05(8) . . ?
O1 U3 U2 167.73(6) 45 . ?
O2 U3 U2 40.82(6) . . ?
O4 U3 U2 117.93(6) 45 . ?
U3 U3 U2 61.151(2) 28 . ?
OW1 Co1 OW1 66.1(5) . 2_565 ?
OW1 Co1 OW2 168.4(3) . 2_565 ?
OW1 Co1 OW2 102.3(3) 2_565 2_565 ?
OW1 Co1 OW2 102.3(3) . . ?
OW1 Co1 OW2 168.4(3) 2_565 . ?
OW2 Co1 OW2 89.3(4) 2_565 . ?
OW1 Co1 O9 91.96(8) . . ?
OW1 Co1 O9 91.96(8) 2_565 . ?
OW2 Co1 O9 88.34(7) 2_565 . ?
OW2 Co1 O9 88.34(7) . . ?
OW1 Co1 O9 91.96(8) . 2_565 ?
OW1 Co1 O9 91.96(8) 2_565 2_565 ?
OW2 Co1 O9 88.34(7) 2_565 2_565 ?
OW2 Co1 O9 88.34(7) . 2_565 ?
O9 Co1 O9 175.32(19) . 2_565 ?
OW1 Co1 OW1A 88.9(4) . 2_565 ?
OW1 Co1 OW1A 22.9(3) 2_565 2_565 ?
OW2 Co1 OW1A 79.4(3) 2_565 2_565 ?
OW2 Co1 OW1A 168.7(3) . 2_565 ?
O9 Co1 OW1A 91.31(5) . 2_565 ?
O9 Co1 OW1A 91.31(5) 2_565 2_565 ?
OW1 Co1 OW1A 22.9(3) . . ?
OW1 Co1 OW1A 88.9(4) 2_565 . ?
OW2 Co1 OW1A 168.7(3) 2_565 . ?
OW2 Co1 OW1A 79.4(3) . . ?
O9 Co1 OW1A 91.31(5) . . ?
O9 Co1 OW1A 91.31(5) 2_565 . ?
OW1A Co1 OW1A 111.8(4) 2_565 . ?
OW4 Co2 OW4 94.5(2) 5 . ?
OW4 Co2 OW4 94.5(2) 5 9 ?
OW4 Co2 OW4 94.5(2) . 9 ?
OW4 Co2 O5 91.77(17) 5 9 ?
OW4 Co2 O5 168.99(18) . 9 ?
OW4 Co2 O5 94.10(16) 9 9 ?
OW4 Co2 O5 168.99(18) 5 . ?
OW4 Co2 O5 94.10(16) . . ?
OW4 Co2 O5 91.77(17) 9 . ?
O5 Co2 O5 78.72(12) 9 . ?
OW4 Co2 O5 94.10(16) 5 5 ?
OW4 Co2 O5 91.77(17) . 5 ?
OW4 Co2 O5 168.99(18) 9 5 ?
O5 Co2 O5 78.72(12) 9 5 ?
O5 Co2 O5 78.72(12) . 5 ?
OW4 Co2 OW3 57.95(16) 5 . ?
OW4 Co2 OW3 57.95(16) . . ?
OW4 Co2 OW3 57.95(16) 9 . ?
O5 Co2 OW3 132.92(8) 9 . ?
O5 Co2 OW3 132.92(8) . . ?
O5 Co2 OW3 132.92(8) 5 . ?
OW4 Co2 Co3 122.05(16) 5 . ?
OW4 Co2 Co3 122.05(16) . . ?
OW4 Co2 Co3 122.05(16) 9 . ?
O5 Co2 Co3 47.08(8) 9 . ?
O5 Co2 Co3 47.08(8) . . ?
O5 Co2 Co3 47.08(8) 5 . ?
OW3 Co2 Co3 180.0(2) . . ?
O5 Co3 O5 77.70(11) 9 . ?
O5 Co3 O5 77.70(11) 9 5 ?
O5 Co3 O5 77.70(11) . 5 ?
O5 Co3 O5 102.30(11) 9 37 ?
O5 Co3 O5 180.00(7) . 37 ?
O5 Co3 O5 102.30(11) 5 37 ?
O5 Co3 O5 180.00(13) 9 45 ?
O5 Co3 O5 102.30(11) . 45 ?
O5 Co3 O5 102.30(11) 5 45 ?
O5 Co3 O5 77.70(11) 37 45 ?
O5 Co3 O5 102.30(11) 9 41 ?
O5 Co3 O5 102.30(11) . 41 ?
O5 Co3 O5 180.0(2) 5 41 ?
O5 Co3 O5 77.70(11) 37 41 ?
O5 Co3 O5 77.70(11) 45 41 ?
O5 Co3 Co2 46.41(7) 9 . ?
O5 Co3 Co2 46.41(7) . . ?
O5 Co3 Co2 46.41(7) 5 . ?
O5 Co3 Co2 133.59(7) 37 . ?
O5 Co3 Co2 133.59(7) 45 . ?
O5 Co3 Co2 133.59(7) 41 . ?
O5 Co3 Co2 133.59(7) 9 37 ?
O5 Co3 Co2 133.59(7) . 37 ?
O5 Co3 Co2 133.59(7) 5 37 ?
O5 Co3 Co2 46.41(7) 37 37 ?
O5 Co3 Co2 46.41(7) 45 37 ?
O5 Co3 Co2 46.41(7) 41 37 ?
Co2 Co3 Co2 180.00(5) . 37 ?
O1 P1 O3 114.34(16) . . ?
O1 P1 O2 113.60(15) . . ?
O3 P1 O2 102.67(14) . . ?
O1 P1 C1 107.67(16) . . ?
O3 P1 C1 109.56(16) . . ?
O2 P1 C1 108.84(16) . . ?
O1 P1 U2 124.15(10) . . ?
O3 P1 U2 51.79(10) . . ?
O2 P1 U2 51.46(9) . . ?
C1 P1 U2 128.17(12) . . ?
C2 C1 P1 110.9(2) . . ?
O4 C2 O5 122.6(3) . . ?
O4 C2 C1 118.8(3) . . ?
O5 C2 C1 118.7(3) . . ?
P1 O1 U3 138.42(15) . 41 ?
P1 O2 U3 139.69(14) . . ?
P1 O2 U2 101.33(12) . . ?
U3 O2 U2 102.70(9) . . ?
P1 O3 U1 151.17(15) . . ?
P1 O3 U2 101.12(12) . . ?
U1 O3 U2 103.81(9) . . ?
C2 O4 U3 137.0(2) . 41 ?
C2 O5 Co2 146.2(2) . . ?
C2 O5 Co3 127.1(2) . . ?
Co2 O5 Co3 86.51(10) . . ?
U2 O9 Co1 177.9(2) . . ?
U2 O12 U1 124.87(7) . 3 ?
U2 O12 U1 124.87(7) . . ?
U1 O12 U1 108.23(14) 3 . ?
U2 O14 U3 123.15(7) . . ?
U2 O14 U3 123.15(7) . 28 ?
U3 O14 U3 113.67(14) . 28 ?
U3 O15 U3 107.89(16) 28 . ?
OW1A OW1 Co1 85.3(8) . . ?
OW1 OW1A Co1 71.9(8) . . ?
OW13 OW8 OW13 129(2) 26 . ?
OW11 OW9 OW11 86(3) 28 . ?
OW13 OW10 OW11 103.1(17) . . ?
OW9 OW11 OW11 46.8(16) . 28 ?
OW9 OW11 OW10 179(2) . . ?
OW11 OW11 OW10 132.0(9) 28 . ?
OW10 OW13 OW8 126(2) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 O6 1.783(4) . ?
U1 O7 1.798(4) . ?
U1 O12 2.266(2) 26 ?
U1 O12 2.266(2) . ?
U1 O3 2.378(2) . ?
U1 O3 2.378(2) 26 ?
U1 O13 2.429(4) . ?
U1 U1 3.6718(3) 3 ?
U1 U2 3.94653(17) 26 ?
U1 U2 3.94653(17) . ?
U2 O8 1.808(3) . ?
U2 O9 1.826(3) . ?
U2 O12 2.186(3) . ?
U2 O14 2.194(3) . ?
U2 O2 2.622(2) 28 ?
U2 O2 2.622(2) . ?
U2 O3 2.632(2) 28 ?
U2 O3 2.632(2) . ?
U2 P1 3.2875(8) 28 ?
U2 P1 3.2875(8) . ?
U2 U3 3.91322(18) . ?
U2 U3 3.91322(19) 28 ?
U3 O11 1.798(2) . ?
U3 O10 1.801(3) . ?
U3 O14 2.2556(18) . ?
U3 O15 2.335(2) . ?
U3 O1 2.336(2) 45 ?
U3 O2 2.385(2) . ?
U3 O4 2.388(2) 45 ?
U3 U3 3.7763(2) 28 ?
Co1 OW1 2.041(7) . ?
Co1 OW1 2.041(7) 2_565 ?
Co1 OW2 2.053(5) 2_565 ?
Co1 OW2 2.053(5) . ?
Co1 O9 2.128(3) . ?
Co1 O9 2.128(3) 2_565 ?
Co1 OW1A 2.140(8) 2_565 ?
Co1 OW1A 2.140(8) . ?
Co2 OW4 2.077(4) 5 ?
Co2 OW4 2.077(4) . ?
Co2 OW4 2.077(4) 9 ?
Co2 O5 2.082(3) 9 ?
Co2 O5 2.082(3) . ?
Co2 O5 2.082(3) 5 ?
Co2 OW3 2.385(6) . ?
Co2 Co3 2.8698(14) . ?
Co3 O5 2.105(3) 9 ?
Co3 O5 2.105(3) . ?
Co3 O5 2.105(3) 5 ?
Co3 O5 2.105(3) 37 ?
Co3 O5 2.105(3) 45 ?
Co3 O5 2.105(3) 41 ?
Co3 Co2 2.8698(14) 37 ?
P1 O1 1.499(3) . ?
P1 O3 1.526(3) . ?
P1 O2 1.533(2) . ?
P1 C1 1.808(4) . ?
C1 C2 1.517(5) . ?
C2 O4 1.251(4) . ?
C2 O5 1.261(4) . ?
O1 U3 2.336(2) 41 ?
O4 U3 2.388(2) 41 ?
O12 U1 2.266(2) 3 ?
O14 U3 2.2556(18) 28 ?
O15 U3 2.335(2) 28 ?
OW1 OW1A 0.835(10) . ?
OW6 OW6 1.201(18) 26 ?
OW7 OW7 1.186(19) 28 ?
OW8 OW13 1.67(3) 26 ?
OW8 OW13 1.67(3) . ?
OW9 OW11 0.87(2) 28 ?
OW9 OW11 0.87(2) . ?
OW10 OW13 1.57(3) . ?
OW10 OW11 1.65(3) . ?
OW11 OW11 1.20(3) 28 ?
